Dec 3, 2018 - Vascular cells isolated from porcine aorta were subjected to ...... aligned microfibers in a rat abdominal aorta replacement model. J. Biomed.
Dec 3, 2018 - It is crucial to understand the cell-material interaction while designing a functional tissue engineered vascular graft. Natural silk biopolymer has ...
Dec 3, 2018 - It is crucial to understand the cell-material interaction while designing a functional tissue engineered vascular graft. Natural silk biopolymer has ...
Jun 21, 2018 - The flow rate was 0.3 Î¼L/min, and the wavelength detection was set at 250 ..... 4.5, and 2.9%, respectively), kaempferol 3-glucoside (2.3, 1.9, and 2.4%, ... after storage at 0 Â°C, but no significant increase in cyanidin 3-glucoside
Jun 21, 2018 - ... Microbiology and Molecular Biology, University of South Florida, 4202 ... Research and Education Center, University of University of Florida, ...
Jun 21, 2018 - Marvin Abountiolasâ , Katrina Kellyâ , Yavuz Yagizâ¡ , Zheng Liâ¡ , Gail Mahnkenâ¡ , Wlodzimierz Borejsza-Wysockiâ¡ , Maurice Marshallâ¡ ...
Jun 21, 2018 - Sensory Quality, Physicochemical Attributes, Polyphenol Profiles, and Residual Fungicides in Strawberries from Different Disease-Control ...
Insect Biology and Population Management Research Laboratory, U.S. Department of Agriculture, Agricultural Research Service, Tifton, Georgia 31794, ...
Chemical and Genetic Attributes of a Maize-Silk Olfactory Trait. N. W. Widstrom,*,â R. A. Flath,â¡ and P. J. Loesch, Jr.Â§. Insect Biology and Population ...
Jump to Results and Discussion - In terms of solar energy conversion, this coarser but bicontinuous nanostructure could be beneficial in electron transport, ...
Surface Patterning and Innate Physicochemical Attributes of Silk Films Concomitantly Govern Vascular Cell Dynamics Prerak Gupta, Joseph Christakiran Moses, and Biman B. Mandal* Biomaterial and Tissue Engineering Laboratory, Department of Biosciences and Bioengineering, Indian Institute of Technology Guwahati, Guwahati-781039, Assam, India
Downloaded via UNIV OF BRITISH COLUMBIA on January 4, 2019 at 16:26:22 (UTC). See https://pubs.acs.org/sharingguidelines for options on how to legitimately share published articles.
S Supporting Information *
ABSTRACT: Functional impairment of vascular cells is associated with cardiovascular pathologies. Recent literature clearly presents evidence relating cell microenvironment and their function. It is crucial to understand the cell-material interaction while designing a functional tissue engineered vascular graft. Natural silk biopolymer has shown potential for various tissue-engineering applications. In the present work, we aimed to explore the combinatorial eﬀect of variable innate physicochemical properties and topographies of silk ﬁlms on functional behavior of vascular cells. Silk proteins from diﬀerent varieties (mulberry Bombyx mori, BM; and nonmulberry Antheraea assama, AA) possess unique inherent amino acid composition that leads to variable surface properties (roughness, wettability, chemistry, and mechanical stiﬀness). In addition, we engineered the silk ﬁlm surfaces and printed a microgrooved pattern to induce unidirectional cell orientation mimicking their native form. Patterned silk ﬁlms induced unidirectional alignment of porcine vascular cells. Regardless of alignment, endothelial cells (ECs) proliferated favorably on AA ﬁlms; however, it suppressed production of nitric oxide (NO), an endogenous vasodilator. Unidirectional alignment of smooth muscle cells (SMCs) encouraged contractile phenotype as indicated by minimal cell proliferation, increment of quiescent (G0) phase cells, and upregulation of contractile genes. Moderately hydrophilic ﬂat BM ﬁlms induced cell aggregation and augmented the expression of contractile genes (for SMCs) and endothelial nitric oxide synthase, eNOS (for ECs). Functional studies further conﬁrmed SMCs’ alignment improving collagen production, remodeling ability (matrix metalloproteinase, MMP-2 and MMP-9 production) and physical contraction. Altogether, this study conﬁrms vascular cells’ functional behavior is crucially regulated by synergistic eﬀect of their alignment and cell−substrate interfacial properties. KEYWORDS: silk ﬁlms, patterning, vascular cell, alignment, cell−substrate interface, surface topography
the way to mimic the 3D complex microenvironments while preserving the easiness of working with 2D surfaces.3,4 At the cell−substrate interface, several factors (including topography, wettability, roughness, chemistry, and mechanical properties of the substrate) play a crucial role in determining cell behavior. The majority of human-adherent cell types are spatially arranged innately in a unique manner that helps them maintain their function and overall tissue dynamics.5,6 Of note, vascular cells, typically endothelial cells (ECs) in tunica interna and smooth muscle cells (SMCs) in tunica media of blood vessels, follow a unique topographical arrangement. ECs are aligned along the direction of blood ﬂow and maintain vascular homeostasis,7 whereas SMCs are aligned radially, contributing to the mechanical robustness and vasoactive responsiveness of blood vessels.8 These design parameters become important for tissue engineering of vascular grafts where the main focus for success is to engineer the scaﬀold wall surface in such a way so
ECM response, a crucial parameter for assembly of cell-matrix adhesion complexes and cell spreading.18 Several studies have reported the eﬀect of individual factor on cellular functionality; however, in a native in vivo microenvironment, cells are exposed to multiple factors simultaneously. Hence, investigating the combinatorial eﬀect of more than one factor becomes of great importance. In the present study, we intend to explore the functionality of vascular cells (ECs and SMCs) when cultured on mulberry Bombyx mori-BM and non-mulberry Antheraea assama-AA silk ﬁlms. Our selection of using diﬀerent silk relied on following crucial parameters: (1) both proteins are highly biocompatible and have been explored for various tissue engineering applications;27−30 (2) their ability to be fabricated into myriad structural designs with nano level accuracy, allowing surface engineering to print any desirable pattern;27 and (3) structural variability in their native amino acid sequence and arrangement of secondary protein structures.31 The molecular composition of these silk proteins is quite diﬀerent. Heavy chain of both silk proteins consists majorly of Ala (44.5% vs 28.8% for AA vs BM) and Gly (30.1% vs 43.7% for AA vs BM), nonpolar amino acids.32 The alanine methyl groups are usually exposed to external microenvironment because of their arrangement outside of protein backbone.33 Because of the presence of diﬀerent percentages of hydrophobic amino acid residues in BM and AA silk proteins, the surface wettability of ﬁlms made of these proteins is expected to be dissimilar. Moreover, AA ﬁlms demonstrate higher roughness as compared to BM ﬁlms.27 The crystalline core of AA is made-up of poly (alanine) motifs, which makes 37.4% of total Ala out of 44.5%. In contrast, BM protein have multiple repeats of AGSGAG comprising 55% of total crystalline core.34 Diﬀerential amino acid composition and arrangement leads to formation of unique secondary structures. For instance, the poly (alanine) motifs present in AA silk prefer to form antiparallel β-sheets via noncovalent intermolecular interactions, which confers tensile strength.35 Besides, it also provides more hydrophobicity, forming stronger β-sheets as compared with AGSGAG repeats of BM silk. In general, alanine motifs provide tensile strength to silk ﬁbers whereas glycine rich sequences are responsible for ﬁber elasticity. It has also been reported that even the short poly(alanine) stretches (A)6 are able to confer remarkable tensile strength to AA protein by forming strong β-nanocrystal, which is much higher than all other wild silk varieties.36 Additionally, AA silk has the intrinsic presence of RGD cell binding motif in its native amino acid structure, making its surface chemically diﬀerent from BM silk.32 Because of these aforementioned characteristics, surfaces of silk ﬁlms obtained from diﬀerent silks provide variable surface characteristics. Therefore, in the current endeavor, we cultured vascular cells on BM and AA silk ﬁlms and looked into their functional behavior in response to combinatorial eﬀect of multiple physicochemical factors acting at the cell−substrate interface.
that it recruits the progenitor vascular cells and provides a congenial microenvironment for their growth and functionality. Recently, several studies have shown the corelation between vascular cell morphology/organization and their functionality in vitro9 and in vivo.10,11 A functional and continuous monolayer of ECs maintains uninterrupted blood ﬂow in the blood vessels. Any damage in the EC monolayer may lead to various pathological conditions such as thrombosis, hyperplasia, stenosis, and inﬂammation in the vessel wall, which alters the vascular tone.12 Besides that, cell morphology, shape, alignment and polarity are also other determining factors that regulate EC functionality.13 Hence, mimicking a nativelike physiological environment becomes a point of interest. ECs present in blood vessels’ lumen lining are exposed to shear stress and cyclic circumferential strain due to continuous blood ﬂow. Under these circumstances, these cells tend to adopt unidirectional alignment along the direction of blood ﬂow. The adjacent multiple layers of SMCs in the vascular wall (tunica media) align themselves radially (perpendicular to the direction of blood ﬂow).8 Recently, several researchers have reported the positive eﬀect of unidirectional alignment on vascular cell functionality. The majority of them focused on either engineering the cell culture surfaces (by printing grooved pattern) or by exposing the cultured cells to the ﬂow shear stress.6,8,14,15 Surface wettability is another important parameter that inﬂuences cell morphology, aﬀecting their functionality.6 It is a well-proven fact that cells prefer to spread better on moderate hydrophilic surfaces.16,17 Limited cell adhesion and spreading was reported on highly hydrophilic surfaces because such surfaces do not allow long-term retention of cell adhesion molecules.18 The biochemical composition of the cell culture matrix or surface chemistry also regulates cell morphology and spreading.19,20 For instance, surface biofunctionalization with cell binding RGD peptide enhances the cell attachment and proliferation via an integrin-mediated (cell adhesion receptor) process.21 Apart from surface patterning (guiding cellular alignment), surface roughness determines the functionality of vascular cells. Cellular response to surface roughness at the microscale is a bit controversial because of the inconsistency noticed throughout several reports. For instance, endothelial cells showed superior growth on the rougher PU-PEG (polyurethane-polyethylene glycol) surface regardless of presence of surface cell adhesion peptides (RGD).22 On the contrary, smoother solvent-casted poly (L-lactic acid) (PLLA) surfaces supported better EC functionality.23 Nanostructured titanium surfaces favorably supported the adhesion of SMCs and ECs.24 Such paradoxical behavior is generally attributed to undeﬁned attributes of surface roughness and needs more speciﬁc deﬁnition that considers diﬀerent nanostructured shapes, spacing between irregularities and sharpness of the peaks.18 Among all cell−substrate interface properties, substrate rigidity is considered least important but was recently identiﬁed as a very crucial factor in determining cell fate. The phenomenon of change in a cell’s chemical microenvironment in response to mechanical signals is called “mechanotransduction”.25 Substrates with the same chemical composition and diﬀerent rigidity have shown to modulate SMCs adhesion.18 Studies have shown that substrates with low rigidity does not allow cellular spreading whereas cells spread better on stiﬀer substrates (depending on cell type).26 One of the plausible explanation of such cellular behavior might be related with imbalance between cell traction forces and corresponding
2. MATERIALS AND METHODS 2.1. Fabrication of Silk Films. Mulberry silk (Bombyx mori BM) and non-mulberry silk (Antheraea assama - AA) proteins were used for this study. Silk ﬁbroin (SF) proteins were obtained by following previously described procedures.27 BM silk was extracted by degumming the cocoons in 0.02 M sodium carbonate followed by dissolution in 9.3 M LiBr and dialysis against distilled water for 72 h with frequent water changes. Non-mulberry AA silk was obtained directly from silk glands of mature ﬁfth instar larvae. The glandular protein was extracted using ﬁne forceps and dissolved in 1% (w/v) B
2.3. Isolation and Culture of Vascular Cells. Smooth muscle cells (SMCs) and Endothelial cells (ECs) were isolated from descending porcine aorta following our previously described protocol.27 In brief, porcine descending aorta was collected from local slaughterhouse and transported in ice cold sterile phosphate buﬀered saline (PBS). Tissue was processed within 1h of collection. Associated fat was removed and the aorta was cut into 1 cm2 pieces followed by digestion with collagenase type 1A (1 mg/mL, SigmaAldrich, U.S.A.) keeping luminal side in contact with the plate surface. These tissue sections were further incubated in a humidiﬁed incubator (95% humidity) at 5% CO2, 37 °C for 1h. Post incubation, the luminal surface was scraped to harvest ECs. From the remaining tissue, a medial layer containing SMCs was isolated from the adventitial layer and digested further in 0.5% collagenase for 8h. Digested tissue was ﬁltered through a cell strainer (70 μm pore size, BD Biosciences, U.S.A.) and cultured in high glucose Dulbecco’s Modiﬁed Eagle’s medium (DMEM, Gibco, U.S.A.) supplemented with 10% (/v) fetal bovine serum (FBS, Gibco, U.S.A.) and 1% (v/v) antibiotic-antimycotic solution (Himedia, India) in a humidiﬁed incubator. After 24h of cell adherence, media was changed to ECGS (endothelial cell growth supplement, recommended concentration in DMEM culture media, Sigma-Aldrich, U.S.A.) for ECs and SMGS (smooth muscle cell growth supplement, 2% v/v in DMEM culture media, Life Technologies, U.S.A.) for SMCs. 2.4. Immunostaining for Vascular Cell Identiﬁcation. Vascular cells isolated from porcine aorta were subjected to immunostaining for cell speciﬁc marker expression. ECs were stained for vWF (Von Willebrand factor) and SMCs were stained for Calponin and αSMA (alpha- Smooth muscle actin) markers. Cells cultured on standard TCP (tissue culture plate) were ﬁxed in neutral buﬀered formalin (NBF, Sigma-Aldrich, U.S.A.) overnight and permeabilized with 0.1% (v/v in PBS) TritonX-100 for 15 min. Cells were further treated with blocking solution (2% w/v bovine serum albumin-BSA in PBS) to prevent any nonspeciﬁc binding. Rabbit primary antibody solution was prepared in blocking solution with the following dilutions: vWF (1:400), Calponin (1:250) and αSMA (1:100). Cells were treated with primary antibody for 1 h at 37 °C followed by FITC tagged anti rabbit secondary antibody treatment (1:500) for 1h. Cell nucleus was stained with Hoechst 33342 (1:1000, Sigma-Aldrich, U.S.A.) and the cellular cytoskeleton was stained with rhodamine phalloidin (1:40, Life technologies, U.S.A.). Cells were given three PBS wash after each successive step. Stained cells were imaged under a ﬂuorescent microscope (EVOS FL, Life Technologies, U.S.A.). 2.5. Proliferation of Vascular Cells Cultured on Silk Films. Silk ﬁlms from each experimental group were cut into circular discs (ϕ 15 mm) and placed in a 24 well tissue culture plate. Films were further sterilized followed by conditioning overnight with culture media (DMEM with 10% FBS). Vascular cells (both ECs and SMCs) were seeded carefully onto these discs at a density of 1 × 105 cells/ cm2 suspended in minimal volume (∼20 μL) of culture media to avoid spillage from the ﬁlms. After initial cell adherence onto silk ﬁlms, 1 mL of culture media was added into each well and plate was kept in humidiﬁed incubator (5% CO2, 37 °C). AlamarBlue (ThermoFisher Scientiﬁc, U.S.A.) dye was used to monitor the cell activity and proliferation following manufacturer’s protocol and as described previously.27 Cell growth was determined at three diﬀerent time points and represented as normalized value of percentage reduction of AlamarBlue. 2.6. Cell Distribution Proﬁle and Orientation Analysis. Phase contrast microscopic images of vascular cells (both ECs and SMCs) cultured on silk ﬁlms were captured using microscope (EVOS FL, Life Technologies, U.S.A.). These images were further processed using MBF ImageJ software (model 1.52a, National Institute of Health, U.S.A.). Cell orientation was calculated by OrientationJ plugin, which is available online (http://bigwww.epﬂ.ch/demo/orientation/). Brieﬂy, captured phase contrast images were converted to 32 bit greyscale type and orientation distribution plugin was used to plot the cell distribution proﬁle with 5% minimum coherency level. Moreover, to visualize the distribution of actin cellular ﬁlaments, cells cultured
sodium dodecyl sulfate (SDS). Protein solution was further dialyzed in Milli-Q water at 4 °C for 4 h. Percentage of silk protein was estimated using gravimetric method and SF protein solution was stored at 4 °C until use. A 2% (w/v) SF solution was used for fabricating silk ﬁlms. Both ﬂat and patterned polydimethylsiloxane (PDMS) molds were prepared as per earlier described techniques.24 Flat molds were fabricated by blending PDMS substrate (Dow Corning Corporation, Midland, MI U.S.A.) with its cross-linker (10:1 w/w ratio) and baking at 60 °C for 4 h. Soft lithography technique was used to prepare microgrooved patterned molds (distance between ridges: 3 μm; groove depth: 200 nm);37 4 × 4 cm2 PDMS molds were used to fabricate ﬁlms by spreading 2 mL of 2% SF protein solution and allowing it to dry at ambient ﬂow conditions overnight. The dried silk ﬁlms were exposed to water vapor annealing in a vacuum desiccator for 6 h at 37 °C. The water-stabilized ﬁlms were detached further from the PDMS molds and stored at 4 °C sterile conditions until further use. The following abbreviations are used henceforth for designating diﬀerent experimental groups: standard tissue culture plate (TCP), B. mori ﬂat ﬁlms (BMF), B. mori patterned ﬁlms (BMP), A. assama ﬂat ﬁlms (AAF), and A. assama patterned ﬁlms (AAP). 2.2. Physicochemical Characterization of Silk Films. Water vapor annealed ﬁlms were analyzed for their surface roughness and topography by atomic force microscopy (Agilent model 5500, U.S.A.). All silk ﬁlms were scanned in noncontact mode with a scanning area of 10 × 10 μm2 at room temperature (RT). WSxM 5.0 Develop 7.0 software was used to calculate various parameters and plotting surface proﬁles of patterned silk ﬁlms. Both ﬂat and patterned silk ﬁlms were observed under FESEM (Zeiss, Sigma) for analyzing their surface morphology. FESEM micrographs were captured after gold sputtering of silk ﬁlms. Water contact angle of ﬂat silk ﬁlms was further investigated by sessile drop technique using contact angle goniometer (Holmarc, India). Water vapor annealed silk ﬁlms of 2 × 2 cm2 were used. An automated microsyringe extruded 3 μL of Milli-Q water droplet onto silk ﬁlm and captured images were processed to determine the contact angle of both ﬂat and patterned silk ﬁlms. Patterned silk ﬁlms were characterized parallel (PAR) and perpendicular (PER) to the direction of microgrooves. A scheme of directions of these analyses is shown in Figure S1. For each ﬁlm, at least three diﬀerent spots were used for calculating the contact angle. Silk ﬁlms were further analyzed to explore their mechanical properties. Only water vapor annealed ﬂat ﬁlms were subjected for this analysis because of their stability in the hydrated conditions in which the analyses were performed. Silk ﬁlm strips (length, 3 cm; width, 1 cm) were used for tensile testing under hydrated conditions using Universal Testing Machine (UTM, Instron 5944, U.S.A.) in a BioPuls bath (with PBS as immersion buﬀer) at 37 °C. Stress−strain curves were obtained at a crosshead speed of 1 mm/min until sample failure. Modulus of ﬁlms was calculated as slope of stress−strain curves. Silk ﬁlms were also subjected for cyclic testing until 10 cycles (5% deformation strain) value at a rate of 1 mm/min. Mechanical analysis of silk ﬁlms was performed for at least n = 4 specimens. Infrared spectra of regenerated silk ﬁbroin solutions (B. mori and A. assama) and water vapor annealed silk ﬁlms of the same were characterized using Fourier transform infrared spectrometer (Shimadzu model: IR Aﬃnity-1S WL) in attenuated total reﬂectance (ATR mode) with germanium internal reﬂection element. Each measurement consisted of 30 scans averaged to yield the spectra (4000−400 cm−1) with a resolution of 2 cm−1. The amide-I spectra (1700−1600 cm−1) was further deconvoluted by taking second derivative of the spectra and ﬁtting Gaussian peaks to determine the secondary structures present in the regenerated silk ﬁbroins and its water vapor annealed ﬁlms. Band assignments for secondary structures were given as follows: α-helices (1650−1658 cm−1), β-sheets (1620− 1640 cm−1), antiparallel β-sheets (1670−1695 cm−1), disordered structures (1640−1650 cm−1), and loops (1660−1680 cm−1) following previous reports.38,39 The deconvoluted spectra were areanormalized and subsequently used to determine the percentage of secondary structures present in the samples investigated. C
ACS Biomaterials Science & Engineering on silk ﬁlms were stained with rhodamine-phalloidin ﬂuorescent dye as described previously and observed under a ﬂuorescent microscope (EVOS FL, Life Technologies, U.S.A.). 2.7. Cell Cycle Analysis. Circular discs of silk ﬁlms (ϕ 3 cm) were sterilized, conditioned in culture media and placed in 6-well tissue culture plate. ECs and SMCs were seeded onto silk ﬁlms with a cell density of 1 × 105 cells/cm2. After 4 days of culture, cells were harvested from silk ﬁlms using trypsin-EDTA (Himedia, India) and analyzed for cell cycle proﬁle. Brieﬂy, cell suspension was ﬁxed in ice cold ethanol followed by 2 washes with PBS. Cells were further treated with 200 μg/mL RNase A (Sigma-Aldrich, U.S.A.) for 1 h to avoid any false positive signal from RNAs. Cells suspension was treated with 40 μg/mL propidium iodide (PI, Thermo Fischer Scientiﬁc, U.S.A.) and kept on ice for an additional 10 min prior to ﬂow cytometry date acquisition. Cell cycle data was acquired in FL2 channel using BD Accuri C6 plus ﬂow cytometer machine equipped with blue laser (488 nm). Data was analyzed on inbuilt BD Accuri C6 software to calculate the percentage of cell population present in each phase of cell cycle. 2.8. Analysis of Functional Gene Expression Using qRT-PCR. Vascular cells cultured on topographically diﬀerent silk ﬁlms were investigated for the expression of functional genes. For this, we studied the expression of endothelial nitric oxide synthase (eNOS)/ angiopoietin 1 (ANGPT1) for endothelial cells and alpha smooth muscle actin (αSMA)/smooth muscle myosin heavy chain (SMMHC) contractile markers for smooth muscle cells. After 4 days of culture, cells were lysed using TRIzol reagent (Sigma-Aldrich, U.S.A.) to isolate the RNA. The cell lysate was centrifuged for 10 min at 13 000 rpm at 4 °C followed by transfer of supernatant to fresh tubes containing chloroform. After 15 min, three distinct layers were observed and tubes were centrifuged again at 13 300 rpm. Upper aqueous layer containing RNA was transferred to fresh tubes and RNA was eluted and puriﬁed by repeated washing with ethanol. RNase free water was used to resuspend the RNA pallet. The extracted RNA was quantiﬁed and processed for reverse transcription using high eﬃciency reverse transcription kit (Applied Biosystems, Invitrogen) and thermal cycler (Takara, Japan). Gene expression proﬁle was further quantiﬁed using Power SYBR Green PCR master mix (Applied Biosystems, Life Technologies, U.S.A.) and real-time PCR machine (Applied Biosystems, Quant Studio 5) following manufacturer’s instructions. Primer sequences of the target genes are mentioned in Table 1.
which is a stable degradation product of NO. Spent media was centrifuged to remove any possible cell debris or particles and 100 μL of supernatant was incubated with equal volume of Griess reagent in a 96-well plate at RT under dark conditions for 15 min. The mixture was read at 540 nm and readings were ﬁtted into standard curve equation (obtained using sodium nitrite) to quantify the amount of NO produced by endothelial cells. 2.9.2. Collagen Production by Smooth Muscle Cells. In order to determine the amount of collagen secreted by SMCs, cells were seeded on diﬀerent silk ﬁlms placed in 6 well plates at a density of 5 × 105 cells/well. After 4 days of culture, the experiment was terminated and Sirius red dye based assay was used to quantify the total collagen content following previously published protocol.29 Silk ﬁlms with cultured SMCs were digested using pepsin digestion buﬀer (1 mg/mL pepsin-Sigma-Aldrich, U.S.A., 0.5 M NaCl and 0.1 M acetic acid, pH 3.0). 100 μL from each digested sample was aliquoted in 96 well plate and allowed to dry overnight at 37 °C. The dried sample layer was further treated with Sirius red dye (1 mg/mL) followed by ﬁxation with saturated picric acid for 1 h. Fixed sample coatings were washed with 0.01 N HCl and dissolved in 0.1 N NaOH. Optical density (O.D.) readings were taken at 550 nm using multiplate reader (Tecan inﬁnite M 200 pro). A standard curve was plotted using rat tail collagen (Sigma-Aldrich, U.S.A.) to determine the total collagen content secreted from SMCs cultured on silk ﬁlms. Furthermore, secreted collagen was normalized with total DNA content quantiﬁed using Quant-iT PicoGreen dsDNA Assay Kit (Thermo Fisher Scientiﬁc, U.S.A.) following manufacturer’s instructions. 2.9.3. Gelatin Zymography. To detect the activity of secreted matrix metalloproteinase (MMP-2 and 9) porcine SMCs at cell density of 6000 cells/cm2 were seeded on diﬀerent ﬁlms and cultured in SMC growth media supplemented with 10% (v/v) FBS. After cells attained conﬂuency, these cell-seeded ﬁlms were incubated in SMC growth media without FBS supplementation for 14 h. The serum starved conditioned media was collected to assess the MMP activity through gelatin zymography following previously published protocols.29 Brieﬂy, 40 μg of protein from serum-starved conditioned media from each group were loaded in each lane and separated in nonreducing conditions using 7.5% (w/v) polyacrylamide separating gel with 4 mg/mL gelatin. After resolving the gel was incubated in renaturation buﬀer [50 mM Tris-HCl, pH 7.5, 1% (w/v) triton X-100 (Sigma-Aldrich, U.S.A.), 5 mM CaCl2 (Sigma-Aldrich, U.S.A.) and 1 mM ZnC4H6O4 (Sigma-Aldrich, U.S.A.)] overnight at 37 °C. The gel was then stained with 0.5% (w/v) Coomassie Brilliant Blue R-250 (Himedia, India) and destained to visualize the gelatinolytic bands, which appeared as clear bands in dark background. The densiometric proﬁling was done using Image-J software (NIH, USA). 2.9.4. Collagen Gel Contraction Assay. the functional contractility attained by porcine SMCs with respect to biophysical cues presented by diﬀerent ﬁlms were assessed using collagen gel contraction assay, following previously published protocols.41 Brieﬂy, porcine SMCs were seeded on diﬀerent ﬁlms at a seeding density of 6250 cells/cm2 and cultured for 4 days in SMC growth media supplemented with 10% (v/v) FBS. Thereafter, the cells were detached using trypsin and resultant cell suspension was seeded on to preformed collagen gels (collagen I, rat tail, Gibco, U.S.A. following the manufacturer’s protocol) in 96-well plate at a density of 1 × 105 cells/mL. After 24 h, the extent of collagen gel contraction was assessed using Image-J by measuring the area of gel before contraction and after contraction. 2.10. Statistical Analysis. All of the statistical analyses were performed using OriginPro 8 (Origin lab Corporation, U.S.A.) following one-way analysis of variance (ANOVA) and Tukey’s test. All the experiments were performed at-least for N = 3, unless otherwise speciﬁed. Signiﬁcant levels were analyzed at 95% and 99% conﬁdence and represented as #p < 0.05 and ##p < 0.01. All data are represented as mean ± standard deviation.
Table 1. Primer Sequences of Target Genes gene porcine eNOS porcine ANGPT1 porcine αSMA porcine SM-MHC porcine GAPDH
2.9. Functional Studies. 2.9.1. NO Production by Endothelial Cells. Production of NO (nitric oxide) by endothelial cells was quantiﬁed as per previously described protocol.40 Circular silk ﬁlm discs were placed in a 12-well tissue culture plate, sterilized, and conditioned with culture media prior to cell seeding. A higher cell number (∼5 × 105) were seeded into each well to obtain a uniform cell monolayer. After day 1 of culture, 1 mL of media was pooled out and replaced with same volume of fresh media. The experiment was terminated after 4 days of culture and spent media was collected in fresh vials. Collected media was stored at −20 °C until further use. Nitrite was quantiﬁed by using Griess reagent (Sigma-Aldrich, U.S.A.)
3. RESULTS 3.1. Physicochemical Properties of Silk Films. Cell substrate interaction inﬂuences the cells’ functionality. Surface D
Figure 1. Surface characterization of silk ﬁlms. (A) Atomic force microscopic images of ﬂat and patterned silk ﬁlms showing surface roughness. Surface plot proﬁle of patterned ﬁlms is also illustrated indicating the groove depth and peak-to-peak distance. (B) FESEM (Field Emission Scanning Electron Microscope) micrographs of silk ﬁlms demonstrating surface topography and patterning. (C) Water contact angles of ﬂat silk ﬁlms (BMF and AAF) and patterned silk ﬁlms (BMP and AAP in both parallel (PAR) and perpendicular (PER) to the microgroove direction). Images show droplet micrographs in contact with silk ﬁlms. Contact angle values mentioned in the table are representative of at least three diﬀerent spots on silk ﬁlm surfaces.
topography is one of the factors that cells experience when cultured on any substrate. Therefore, we performed AFM scanning of silk ﬁlms (Figure 1A). A considerably higher surface roughness was noticed for AAF ﬁlms ranging 57.52 ± 3.89 nm, approximately 1.6 times more than BMF ﬁlms. Reported values are representative of 3 diﬀerent scanning spots. When calculated for patterned silk ﬁlms (BMP and AAP), no such roughness diﬀerence was observed and the patterning (microgroove pattern) dominated the nano range roughness diﬀerence. The surface plot of patterned silk ﬁlms demonstrated smoother ends of microgrooves for BMP whereas irregular edges were observed for AAP ﬁlms. Distance between consecutive microgroove ridges was recorded to be ranging from 2.8−3.0 μm for both type of patterned ﬁlms. Similar features were observed when these ﬁlms were visualized under FESEM (Figure 1B). AA ﬁlms showed
rougher surface, whereas smoother surface and edges were observed for BM ﬁlms. Another crucial determining factor is surface contact angle or surface hydrophobic/hydrophilic nature that governs cellular adhesion, spreading and functionality. We further investigated the water contact angle for both of silk protein types. Both silk ﬁlms were hydrophilic because of the fact that their water contact angles were well below 90°; however, their degree of hydrophilicity was signiﬁcantly diﬀerent. BMF ﬁlms showed approximately 1.43 times higher contact angle as compared to AAF ﬁlms, making it moderately hydrophilic than AAF type (Figure 1C). We further analyzed the contact angles for patterned silk ﬁlms along and perpendicular to the direction of microgrooves. Again, a similar trend was observed and AAP ﬁlms showed relatively higher degree of hydrophilicity with less contact angle. The contact angle values for various silk ﬁlms are summarized in Table 2. E
annealing, a blue shift was observed in the amide I region. Alternatively, amide II and amide III regions demonstrated a red shift, a characteristic of β-sheet transition after water vapor annealing, making silk ﬁlms water-stable.27,42 To quantify the secondary structure composition in silk solution and water stable silk ﬁlms, we deconvoluted the amide I region between 1600 and 1700 cm−1 region (Figure 3B). The percentage of secondary structures after water vapor annealing is summarized in Table 3. The blue shift noticeable in the amide I spectra of water annealed ﬁlms meant an increase antiparallel β-sheet and cumulative β-sheet content was much higher than in ﬁbroin solution indicating water stability of ﬁlms consistent with previous reports. The higher percentage of β-sheet in nonmulberry silk is attributed to the poly (alanine) present in A. assama. 3.2. Marker Analysis of Vascular Cells and Their Proliferation on Silk Films. Vascular cells isolated from porcine descending aorta were identiﬁed based on expression of cell speciﬁc markers. ECs expressed uniformly distributed typical dotted pattern of von Willebrand Factor (vWF) in cytosol−a glycoprotein produced by endothelial cells. SMCs on the other hand showed expression of two signature protein markers: αSMA (alpha smooth muscle actin−early diﬀerentiation marker) and calponin (mid diﬀerentiation marker) (Figure S3). The presence and predominant expression of speciﬁc markers conﬁrmed the vascular cell identity. We further investigated the vascular cell proliferation on silk ﬁlms, taking a ﬁrst step toward assessment of cell−material interaction. Both SMCs and ECs were compatible with diﬀerent silk ﬁlm surfaces and they we metabolically active for whole examination period. In all experimental groups, normalized alamar reduction value increased from day 1 to day 6 (p < 0.01), attesting the active cell proliferation; however, variable growth patterns were observed for diﬀerent silk ﬁlms. Utmost growth of ECs on day 6 was observed on AA ﬁlms
Table 2. Contact Angles of Silk Films sample BMF AAF BMP PAR BMP PER AAP PAR AAP PER
contact angle (in deg) 66.92 46.76 68.41 64.98 40.93 39.58
± ± ± ± ± ±
1.75 1.39 1.28 1.56 1.02 1.87
Furthermore, mechanical properties of silk ﬁlms were analyzed. Only water-vapor-annealed ﬂat silk ﬁlms were subjected to this analysis. Stress−strain curves suggested higher slope of AAF ﬁlms as compared with BMF (Figure 2A). The representative load−displacement curves are also shown in Figure S2. AAF ﬁlms were stronger/stiﬀer and showed ∼2 fold higher modulus (32.54 ± 9.51 MPa) than BMF ﬁlms (16.79 ± 0.51 MPa) (Figure 2B, p < 0.01). A similar trend was observed for stress at failure (3.09 ± 0.65 MPa vs 8.54 ± 1.04 MPa for BMF vs AAF ﬁlms respectively) (Figure 2C, p < 0.01); however, no signiﬁcant diﬀerence was observed for strain at failure (0.25 ± 0.08 MPa vs 0.30 ± 0.12 MPa for BMF vs AAF ﬁlms respectively)(Figure 2D). Tensile cyclic testing of silk ﬁlms was also performed to obtain hysteresis behavior. BMF ﬁlms did not exhibit much of energy loss between ﬁrst and last cycle (Figure 2E); however, strain hardening and energy gain was observed for AAF ﬁlms until ﬁfth cycle followed by plateau for last ﬁve cycles (Figure 2F). Chemical structure analysis was further performed to investigate the secondary structure composition of silk ﬁlms (Figure 3A). Silk ﬁbroin solution (AAS and BMS) and water vapor annealed ﬁlms (AAF and BMF) were subjected for this analysis. All specimen showed characteristic peaks in amide I (1610−1660 cm−1), amide II (1510−1560 cm−1), and amide III (1210−1260 cm−1) regions.27 On comparing the samples before (AAS, BMS) and after (AAF, BMF) water vapor
Figure 2. Mechanical properties of silk ﬁlms. (A) Representative stress−strain curves showing the slope of BM and AA ﬂat hydrated ﬁlms. (B) Modulus of silk ﬁlms calculated from stress−strain curve slope. (C) Comparison of stress at failure values for both silk ﬁlms. (D) Comparison of strain at failure values for both silk ﬁlms. (E) Representative tensile cyclic analysis of BM silk ﬁlms. (F) Representative tensile cyclic analysis of AA silk ﬁlms. (##p < 0.01, n.s.: not signiﬁcant). F
Figure 3. Fourier Transform Infrared (FTIR) spectra of silk ﬁlms. (A) Spectrographs showing peak shifts in amide I, II, and III peaks before and after β-sheet induction: BM solution (BMS), AA solution (AAS), ﬁlms after β-sheet induction (BM ﬁlm (BMF), AA ﬁlm (AAF)). (B) Deconvulution of amide I peaks to determine secondary structure through second order derivative of amide I spectra for (i) BMS, (ii) AAS, (iii) BMF, and (iv) AAF.
than ﬂat surfaces respectively (p < 0.01), a clear indication toward dominant eﬀect of cell alignment (Figure 4B). 3.3. Vascular Cell Distribution on Diﬀerent Silk Films. Multiple factors that aﬀect the cellular distribution include surface roughness, surface hydrophilicity, surface patterning, and extent of cell−cell/cell-surface interaction depending upon cell seeding density. All these factors concomitantly regulate the cell spreading and distribution; which ultimately determine cellular function. Here in this study we tried to analyze the vascular cell distribution pattern on topographically diﬀerent silk ﬁlms. ECs arranged themselves in their signature cobblestone morphology on TCP. When cultured on silk ﬁlms, cell elongation was observed but still most of the cells were distributed uniformly and spread well on all silk ﬁlms except BMF, where slight cell clustering was observed (Figure 5A). On a similar note, SMCs followed the same distribution pattern and predominant clustering of cells was observed after 4 days of culture on BMF ﬁlms (Figure 5B). Even in certain cases, where SMCs cultured on BMP ﬁlm, clustering tended to dominate the cellular alignment. Cell orientation proﬁles were also plotted to ensure unidirectional cell alignment. Both ECs
Table 3. Eﬀect of Water Vapor Annealing on Silk Secondary Structure Composition percentage (%) secondary structures
irrespective of their surface topography, it was signiﬁcantly higher than standard tissue culture plate (TCP), and both of BM silk ﬁlm types (p < 0.01). ECs’ proliferation on AAP was 1.52 times higher than BMP counterpart and 1.27 times higher than TCP (Figure 4A). SMCs exhibited a completely diﬀerent growth proﬁle on day 6 and patterning of these cells led to slower proliferation. No signiﬁcant diﬀerence was observed among any of the ﬂat surfaces (AAF, BMF, and TCP). SMCs proliferation on AAP and BMP was 1.15 and 1.58 times slower
Figure 4. Proliferation of vascular cells on silk ﬁlms. Proliferation proﬁle of (A) ECs and (B) SMCs cultured on silk ﬁlms (##p < 0.01). G
Figure 5. Orientation proﬁle of vascular cells cultured on silk ﬁlms. Phase contrast microscopic images of (A) endothelial cells and (B) smooth muscle cells cultured onto tissue culture plate (TCP) and silk ﬁlms after 4 days. Images were processed using ImageJ software to calculate the cell distribution/orientation proﬁle. Black arrows are indicating the direction of cellular alignment. (C) Orientation of cytoskeletal actin ﬁbers. Cells cultured onto silk ﬁlms were stained with rhodamine-phalloidin to investigate the distribution of actin ﬁbers. Unidirectional alignment of actin ﬁbers was observed for cells cultured onto patterned silk ﬁlms (AAP and BMP). White arrows are indicating the direction of cellular alignment. H
Figure 6. Analysis of cell cycle. Vascular cells cultured on silk ﬁlms were subjected for cell cycle analysis after 4 days. Cell cycle proﬁle of (A) endothelial cells and (B) smooth muscle cells, showing four distinct phases (G0, G1, S, and G2/M). Percentage population of cells in each phase is represented for (C) endothelial cells and (D) smooth muscle cells. (n.s.: not signiﬁcant, ##p < 0.01, #p < 0.05).
noticed for cells growing on patterned silk ﬁlms irrespective of other surface properties (p < 0.01). Approximately 30 and 38% of the total cell population was trapped in the G0 phase for BMP and AAP ﬁlms groups respectively (Figure 6D). 3.5. Real Time Gene Expression Proﬁle of Vascular Cells. The eﬀect of cell morphology and distribution at gene level was analyzed by quantifying the real-time gene expression after 4 days of culture. We investigated ECs’ function speciﬁc genes: eNOS (encodes for an enzyme involved in synthesis of NO, a key molecule determining the blood vessel dynamics) and Angiopoietin 1 (crucial modulator of vascular development and angiogenesis). eNOS expression in ECs was surprisingly found to be boosted for cells cultured on BMF (∼19 times higher) as compared to all other experimental groups except TCP (p < 0.01) (Figure 7A). Minimal expression of eNOS was observed for ECs cultured on AAP ﬁlms. Expression proﬁle of ANGPT1 gene was inﬂuenced by cellular patterning. Alignment of ECs on patterned silk ﬁlms (BMP and AAP) downregulated the ANGPT1 expression by almost 50 times compared to that for ﬂat ﬁlms (BMF and AAF) and TCP (p < 0.01) (Figure 7B). We further analyzed the gene expression proﬁle of SMCs cultured on silk ﬁlms. Two functional genes were selected for this study; αSMA − early diﬀerentiation marker and SM-MHC (smooth muscle
and SMCs were able to align themselves following the surface patterning as their unidirectional pattern is attested by single peak on the orientation curve; whereas cells cultured on ﬂat silk ﬁlms and TCP exhibited a random distribution and multiple peaks throughout the orientation angle range (Figure 5A, B). We further stained the cellular cytoskeleton with rhodamine-phalloidin ﬂuorescent dye to analyze the actin ﬁlament distribution pattern. Actin ﬁlaments also followed the similar pattern and unidirectional alignment was observed on patterned silk ﬁlms (Figure 5C). Representative lower magniﬁcation images of vascular cells cultured on various silk ﬁlms are shown in Figure S4. 3.4. Cell Cycle Analysis. Earlier reports demonstrate the connection between expression of speciﬁc genes and cell cycle progression.43 Hence, we looked further into cell cycle phases of vascular cells cultured on silk ﬁlm surfaces with variable topographies. Cell cycle proﬁle of ECs and SMCs is shown in Figure 6A, B, respectively, indicating diﬀerent cell cycle phases with assorted colors. On quantifying the percent population of vascular cells present in each phase, we did not observe any signiﬁcant diﬀerence in G0 phase for ECs. However, on comparing the G1 phase population, higher percentage of cells was observed (Figure 6C). In contrast, on analyzing for SMCs, a signiﬁcantly higher quiescent phase population (G0) was I
Figure 7. Quantiﬁcation of functional gene expression by qRT-PCR. Vascular cells cultured on silk ﬁlms were investigated for functional gene expression after 4 days of culture. Endothelial cells were tested for (A) eNOS and (B) ANGPT1 expression, whereas smooth muscle cells were tested for (C) αSMA and (D) SM-MHC expression. (#p < 0.05, ##p < 0.01).
Figure 8. Production of functional moieties by vascular cells cultured on silk ﬁlms. (A, B) Endothelial cells were tested for production of NO (Nitric oxide) from day 1 to day 4. (C, D) Total collagen content produced by smooth muscle cells was also quantiﬁed which was further normalized with DNA content. (n.s.: not signiﬁcant, #p < 0.05, ##p < 0.01).
myosin heavy chain) − late diﬀerentiation marker. Expression of these two genes is related with regulation of SMCs’ phenotype and their contractile behavior. Expression of both genes was upregulated for cells cultured on BMF ﬁlms. αSMA expression was almost 15 times higher as compared to ﬂat AAF
and TCP surfaces and approximately 5 times higher than patterned ﬁlms (p < 0.01). Patterning of SMCs clearly improved the αSMA expression (Figure 7C). As it is the late diﬀerentiation marker, very minimal expression of SM-MHC was observed for ﬂat surfaces (AAF and TCP) post 4 days of J
Figure 9. Functional analysis of smooth muscle cells. (A) Representative gelatin zymography proﬁle of SMC media collected after 4 days of culture period showing the expression of MMP2 and MMP9 enzymes. (i) Image showing MMP bands in diﬀerent groups. Quantiﬁcation of band intensity of (ii) MMP-9 and (iii) MMP-2 representing relative expression. (B) Collagen gel contraction assay of smooth muscle cells. (i) SMCs were entrapped in collagen gel and images were captured at diﬀerent time points. (ii) Quantiﬁcation of gel contraction by measuring the gel size after 24 h. (##p < 0.01).
culture and relatively lower expression was noticed for patterned ﬁlms (BMP and AAP), dictating the eﬀect of cellular patterning on functional gene expression proﬁle (Figure 7D). 3.6. Functional Assessment of Vascular Cells. Expression of functional proteins by tissue speciﬁc cells is one of the crucial requirements for maintaining healthy tissue dynamics. Vascular ECs produce nitric oxide (NO) by calcium-calmodulin dependent enzyme eNOS, an essential regulator of vascular cell growth and protecting blood vessel from adverse eﬀects of platelets.44 Herein, we quantiﬁed the production of NO from ECs cultured on diﬀerent silk ﬁlms on day 1 and day 4. On quantifying the NO production on day 1, cells cultured on TCP showed the maximum NO production signiﬁcantly higher than other experimental groups (p < 0.01). BMP cultured cells produced minimal NO after 4 days (Figure 8A). Interestingly, when we calculated the fold increase proﬁle from day 1 to day 4, we observed the downregulation of NO secretion from aligned ECs (p < 0.01). A paradoxical behavior was observed for TCP cells where NO production was in the range of aligned ECs (Figure 8B). Collagen secretion from SMCs is another parameter we considered for analyzing the cellular functionality. Majority of blood vessel’s ECM is made-
up of collagen and elastin, which help maintain tissue’s mechanical integrity without compromising its elasticity.45 Hence, we quantiﬁed the total collagen secreted from SMCs cultured on various silk ﬁlms at diﬀerent time points. No signiﬁcant diﬀerence was observed for day 1 samples; however, on day 4, cellular alignment induced the collagen production as compared with ﬂat surface cells (Figure 8C). In order to get more accurate idea about collagen secretion, we normalized the total collagen content with DNA. SMCs cultured on AAP produced the maximum collagen and it was signiﬁcantly higher than its counterpart AAF (p < 0.01). However, we did not observe any diﬀerence among BMP and BMF cultured SMCs (Figure 8D). Apart from providing mechanical robustness to the blood vessels by secreting the structural components, SMCs also contribute to tissue remodeling by secreting ECM degrading enzymes- MMP-2 (matrix metalloproteinase-2) and MMP-9. Considering this, we explored the eﬀect of surface topography and hydrophilicity on matrix remodeling capability of SMCs. Our gelatin zymography results suggested that cellular alignment on patterned silk surfaces boost the secretion of MMP-2 and MMP-9 irrespective of cell surface hydrophilicity. Very bright and sharp gel bands were spotted for MMP-2 (at K
blood. Because of direct contact with bloodstream, ECs are regularly exposed to ﬂuid shear stress. It induces their alignment along the direction of blood ﬂow and ultimately help them maintaining their function.13,51 To assess the cumulative eﬀect of surface physicochemical properties and unidirectional cell alignment, we used ﬂat and micro grooved silk ﬁlms from both silk varieties (Figure 1). Surface roughness of AA ﬁlms was superior to BM counterparts as depicted by AFM analysis. The higher surface roughness might be attributed to distinct presence of inherent amino acid stretches and their arrangement.32,33 In contrast, for patterned ﬁlms, no signiﬁcant diﬀerence was observed between two silk types; possibly due to dominance of microstructural surface features over nanostructures. By convention, any surface with a water contact angle less than 90 deg is considered hydrophilic. BMF and AAF ﬁlms showed diﬀerent degrees of hydrophilicity (water contact angle 69.92 ± 1.75 and 46.76 ± 1.39°, respectively). AAF surfaces were more hydrophilic than BMF surfaces. One plausible justiﬁcation for AA surfaces being more hydrophilic might be related with the presence of higher percentage of Ala amino acid residues, which is more hydrophobic than Gly. When in aqueous solution, the nonpolar amino acids tend to form hydrophobic core, leaving polar amino acid residues in contact with outer environment, hence more hydrophilic surface.27 This hypothesis was further substantiated from our FTIR deconvolution data, wherein we observed higher β-sheet content in AA groups in comparison to BM groups. The βsheet-rich crystalline region in silk ﬁbroin forms the intact hydrophobic core. The predominantly higher β-sheet content noticed in AAF contributes for more polar groups exposed outward, which favored the relatively hydrophilic surface of AAF. We further analyzed the contact angle for patterned silk ﬁlms. For more precise measurement, we recorded the contact angle from both directions, i.e., parallel and perpendicular to the microgrooves. A similar hydrophilicity trend was recorded for patterned silk ﬁlms with no signiﬁcant diﬀerence between the contact angles from two diﬀerent directions. Silk ﬁlms’ hydrophilicity range is also relevant for this study because of better EC adhesion on surfaces with a contact angle 40−45° as compared to surfaces with a contact angle of 60−65°.54,55 Although these prior studies report the cell adhesion percentage on surfaces with diﬀerent wettability, the functional behavior of ECs was not investigated. On further analysis of mechanical properties of silk ﬁlms, both ﬁlm types showed signiﬁcant diﬀerence. AA ﬁlms were mechanically stiﬀer and showed higher tensile modulus. Load−displacement curves also suggested signiﬁcantly higher elongation of AA ﬁlms at the breaking point (Figure S3). The higher tensile strength and elongation of AA silk is because of presence of distinct polyalanine stretches in its native structure; conferring formation of higher amounts of antiparallel β-sheet structures (Table 3).35 We further evaluated the biological reaction of vascular cells in response to variable cell−substrate interface features of silk ﬁlms. We ﬁrst looked into the proliferation of vascular cells. Surface-pattern-induced EC alignment is reported to enhance the cellular proliferation56,57 but in the present study, regardless of surface patterning, ECs cultured on AA ﬁlms showed signiﬁcantly higher proliferation than BM ﬁlms in a 6day experiment (p < 0.01) (Figure 4A). As mentioned earlier, interactions at the cell−substrate interface determine the cell behavior; therefore, superior proliferation of ECs on AA ﬁlms
62 kDa) as compared with MMP-9 (92 kDa) (Figure 9A-i). On quantifying the relative band density for MMP-9, TCP cultured cells showed minimal secretion, followed by ﬂat ﬁlms (3 times higher) and patterned ﬁlms (8−9 times higher) (Figure 9A-ii). Similarly, SMCs cultured on TCP showed minimum MMP-2 production and AAP with maximum production of MMP-2 (3 times higher) (Figure 9A-iii). Blood vessel walls are always exposed to continuous contraction and relaxation; hence the most important aspect for SMC functionality is their contractile behavior. To speculate about the impact of diﬀerent surface topography and hydrophilicity on SMCs contractile behavior in 3D culture conditions, we encapsulated SMCs in collagen hydrogels after 4 days of 2D culture on silk ﬁlm surfaces (Figure 9B-i). Gel contraction was quantiﬁed in terms of its size after 24 h culture. Maximum contraction was observed for BMP and AAP groups (∼60%), which was signiﬁcantly higher than ﬂat ﬁlm surfaces (∼30%) and TCP (∼10%) (p < 0.01) (Figure 9B-ii). SMC contraction was solely found to be aﬀected by cellular patterning, and no eﬀect was observed for variable surface hydrophilicity.
4. DISCUSSION There is great interest to understand the eﬀect of physical factors (including surface topography, hydrophilicity and shear stress) on vascular cell functionality.6,8,15 Published reports clearly ensure that chemical factors are not the only regulator for cells’ functional modulation rather physical cues are of equal importance. In this study, we investigated the functional behavior of vascular cells cultured on ﬁlms fabricated using diﬀerent silk (AA and BM). Both silk proteins have unique amino acid sequences, and hence, diﬀerent structural arrangements conferring variable surface properties. Our selection of using silk protein also relied on its remarkable biocompatibility and its ability to acquire any topographical shape even at micro and nano scale, which provides another dimension to add one more variable at cell−substrate interface apart from their natural traits. By using proteins from diﬀerent variety of silk worms (either mulberry or non-mulberry), we fabricated surfaces having diﬀerent properties without any chemical modiﬁcation. These inherent physicochemical properties of BM and AA silk ﬁlms owing to the compositional diﬀerence of the silk ﬁbroins, provided surfaces with variable roughness, wettability, chemistry (presence of RGD motif on AA ﬁlm) and stiﬀness (BMF and AAF). Moreover, we also engineered the silk surfaces by printing a microgroove pattern to induce unidirectional alignment of porcine primary vascular cells. Several studies have recently reported the unidirectional alignment of SMCs6,14,15,46−48 and ECs.7,13,49−52 The rationale behind using such speciﬁcally designed topographical surfaces is to improve the cell functionality. SMCs are capable of adopting two contrasting phenotypes: contractile and synthetic. Cell behavior in both of these phenotypes diﬀers drastically. Under healthy physiological conditions, SMCs remain in the contractile phenotype. However, a phenotype switch (toward synthetic) leads to development of multiple pathological conditions including atherosclerosis, intimal hyperplasia and restenosis after angioplasty. Unidirectional alignment of SMCs is primarily aimed to induce contractile phenotype in order to prevent the diseased condition.53 In blood vessels, ECs’ monolayer in the lumen works as barrier between blood and underlying tissue. It also acts as natural anticoagulant surface that allows uninterrupted channeling of L
observed for endothelial cells cultured on aligned nanoﬁbers and exposed to orthogonal shear stress.63 Such observations clearly indicate that modulation of cell−substrate interface might not be enough to recapitulate the in vivo like microenvironment, and that ﬂuid shear stress is equally important. The functional aspect of vascular cells is further assessed by investigating the expression of functional genes and proteins. A healthy monolayer of ECs is needed to maintain the vascular homeostasis by releasing nitric oxide (NO), which regulates vasodilation and suppresses platelet activation and aggregation.64 The NO molecule is synthesized by nitric oxide synthase (eNOS) enzyme. On analyzing the eNOS expression by ECs cultured on diﬀerent silk ﬁlms, we observed that BMF group showed the maximum expression while the patterned surfaces were found to suppress the eNOS expression (Figure 7A). To further verify at the protein level, we quantiﬁed the production of NO by ECs. TCP cultured ECs produced maximum NO, but to normalize these values, we calculated the fold increase in NO production from day 1 to day 4. In agreement with the gene expression data, a maximum fold increase was observed for the BMF group (p < 0.01) (Figure 8A, B). This is in contrast with previous reports where shear stress was observed to induce eNOS expression and NO production.49 In a previous report, it was observed that substrate compliance induced modulation of ECs’ NO production is mediated by ﬂuid shear stress.65 Surface microgroove induced alignment of ECs has also shown to inﬂuence the production of NO. As suspected in a previous report, microgroove size also matters when it comes to alignment induced functional manipulation of ECs. Microgrooves measuring 5 μm suppressed the eNOS expression signiﬁcantly as compared to higher dimensions.66 In addition, eNOS expression remained unchanged on ﬂat and microgrooved surfaces.66,67 In yet another report, researchers have shown the eﬀect of ratio of groove to ridge width inﬂuencing the ECs’ cytokine and chemokine proﬁle related with remodeling and inﬂammation.49 It is obvious from the prior studies that microgroove dimension also aﬀects ECs’ functionality crucially. The suppressed expression of eNOS and downregulation of NO production from ECs cultured on patterned silk surfaces might be related with the microgroove width of patterned silk ﬁlms used in this study. However, an in depth investigation on eﬀect of microgroove dimensions on silk ﬁlms is needed to ascertain any such possibility. Angiopoietins are another class of proteins that regulate the vascular homeostasis. Angiopoietin-1 (ANGPT1) stabilizes the vascular endothelium by activating Tie2 receptor whereas Angiopoietin-2 (ANGPT2) acts as an antagonist for the former protein.68 Considering the importance of ANGPT1 for the maintenance of healthy vascular endothelium, we further enquired if its expression is aﬀected by surface physicochemical cues of silk ﬁlms. A drastic downregulation of ANGPT1 was observed on patterned silk ﬁlms (Figure 7B). As per our best understanding, there is no such report investigating the eﬀect of biophysical factors on ANGPT1 expression. A detailed molecular analysis is needed to justify these observations. Such paradoxical behavior might be related to the fact that ECs’ alignment and other substrate properties (roughness, wettability, and chemistry) are not the only determining factors of cell functionality; dynamic microenvironment created by blood ﬂow shear stress is also of crucial importance.
might be attributed to either surface wettability (allowing better cell adhesion),54,55 the presence of inherent RGD cell binding motifs on the surface of AA ﬁlms (improving cell adhesion and proliferation),32,58 or substrate stiﬀness (stiﬀer substrates are reported to support better ECs proliferation).59 As suggested by AFM data, AAF and AAP ﬁlms’ surface roughness showed no signiﬁcant diﬀerence, eliminating the inﬂuence of roughness factor on ECs’ proliferation (Figure 1A). These ﬁndings suggest that favorable substrate chemistry, wettability and stiﬀness of AA ﬁlms cumulatively dominate the inﬂuence of surface patterning and subsequent cell alignment on ECs’ proliferation. When compared between BMF and BMP ﬁlms, surface patterning altered the ECs’ proliferation proﬁle. ECs cultured on BMP ﬁlms showed comparatively lesser proliferation. This contrasts with a few prior reports, where ECs’ alignment was found to improve cellular proliferation.56,57 The plausible reason for such cellular behavior might relate with the size of grooves (depth and peak distance) that might alter cell adhesion and proliferation. On the other hand, the proliferation proﬁle of SMCs showed a contrasting behavior than ECs and surface pattern induced alignment was observed to be the dominating factor over other surface properties (Figure 4B). In line with the previous reports, SMCs’ alignment suppressed the proliferation rate, one of the features observed during phenotype transition from synthetic (high proliferation index) to contractile (low proliferation index).53 The underlying mechanism of alignment-induced switch of SMCs’ contractile phenotype has not been explored in details but several studies suspect the possible role of integrin for signaling across the plasma membrane. The two downstream signaling molecules FAK (focal adhesion kinase) and ERK (extracellular signal regulated kinase) might be involved with proliferation alteration of SMCs cultured on ﬂat and patterned surfaces.46 The progression of cell cycle is directly corelated with cell proliferation.53,60 On that account we further investigated the cell cycle proﬁle of vascular cells under the inﬂuence of various surface properties. In native blood vessels, SMCs remain in a nonproliferative quiescent state (G0 phase) and maintain a contractile phenotype.61 Hence, we evaluated the percentage cell population in G0 phase only. SMCs cultured on patterned silk surfaces (BMP and AAP) showed increment in quiescent phase (G0 phase) cell population when compared with ﬂat surface counterparts (p < 0.01). Based on these results, it may be inferred that unidirectional alignment of SMCs induce the nonproliferative (contractile) phenotype via induction of quiescent phase cells. On the other hand, no signiﬁcant diﬀerence was observed for G0 phase cell population for ECs in response to variable cell−substrate interfacial properties. However, in line with proliferation data, a higher G1 phase cell population was recorded for ECs cultured on AA ﬁlms, irrespective of their surface patterning (Figure 6C). It suggests that on AA ﬁlms, more number of cells are entering in cell cycle leading to higher proliferation. Important to note here is that under in vivo conditions, ECs are exposed to a very dynamic microenvironment where they are attached as a monolayer on basement membrane (topographical factor) and remain in direct contact with blood ﬂow (dynamic mechanical loading).62 Both of these factors synergistically modulate the ECs’ cell cycle progression. It is evidenced by a previous report where 3-fold reduction (compared to randomly aligned cells) in Ki67 expression (a proliferation associated protein expressed during cell cycle phases but absent from G0 phase) was M
Our ﬁndings in this work suggest that depending on cell type, surface properties of silk ﬁms synergistically determine cellular functionality. Most of the prior research is focused on extrapolating the eﬀect of a single factor at the molecular level in a highly controlled microenvironment, unveiling that the eﬀect of complex dynamic environment is of much clinical relevance. Although this study is limited to a few standard substrate properties of silk ﬁlms without any consideration of dynamic mechanical microenvironment (because of blood ﬂow shear stress), a detailed molecular and functional analysis by mimicking the complex native-like microenvironment is much needed to understand the vascular cell dynamics under various physio pathological conditions.
SMCs present in tunica media primarily hold the mechanistic responsibility by maintaining their contractile phenotype and producing extracellular matrix (ECM) proteins−collagen and elastin. Therefore, we further aimed to investigate the expression of contractile phenotype related genes and collagen synthesis in response to variable cell− substrate interfacial properties. Expression of two contractile genes is studied, αSMA and SM-MHC. Cellular alignment on patterned surfaces (BMP and AAP) upregulated the expression of both contractile genes, which is in agreement with previous reports.27 However, the BMF group (having a comparatively less hydrophilic surface, lesser surface roughness and without any presence of RGD cell binding motifs) also exhibited the enhanced expression of both of these genes (Figure 7C, D). Such behavior of SMCs might be related to the cell clustering and self-assembly of cells on BMF ﬁlms (Figure 5). Becauseof the inferior hydrophilicity of BMF ﬁlms, after reaching an optimal cell density, SMCs favored more cell−cell interaction compared to cell−substrate interaction and started forming cell clusters mimicking 3D micro tissues that might be one of the plausible justiﬁcations for improved contractile gene expression on BMF ﬁlms.69−71 A similar trend is observed with the collagen quantiﬁcation analysis. Including patterned silk ﬁlms (BMP and AAP); SMCs cultured on BMF ﬁlms showed enhanced collagen production (Figure 8C, D). Increased collagen production from SMCs expressing upregulation of contractile genes is in agreement with a previous report.72 The underlying mechanism for such cellular behavior relies on increased gap junction communication mediated by Wnt3a and subsequent modulation of Wnt signaling.72 Our ﬁndings suggest that although surface-patterning-induced cellular alignment is suﬃcient to induce SMCs’ contractile phenotype and collagen production, other surface properties cumulatively might also lead to a similar cellular response. The functional aspect of SMCs is further elaborated and investigated in terms of their matrix remodeling capability (production of matrix metalloproteinase − MMP-2 and MMP9) and physical contraction ability using collagen gels (Figure 9). For any tissue engineered vascular graft (TEVG), matrix remodeling is very crucial. In this regard, SMCs are known to produce MMP-2 and MMP-9 in blood vessels undergoing remodeling post injury.73 Increased expression of MMP-2 and MMP-9 is observed for BMP and AAP groups independent of other surface properties. Cell alignment induced upregulation of MMPs might relate to the SMCs’ contractile phenotype.72 We further looked into the contraction ability of SMCs cultured on diﬀerent silk ﬁlms by encapsulating them in collagen hydrogel.41 SMCs cultured on patterned surfaces showed better contraction capability (Figure 9B). However, the superior expression of contractile genes for BMF group is not reﬂected here. It indicates that SMCs’ alignment and cell− cell gap junction mediated communication is important for their functional contractile behavior. These outcomes indicate that predominant unidirectional alignment of SMCs lead to induction of their contractile phenotype, allows more collagen and MMP production and shows better contraction capability when compared with cells cultured on ﬂat silk ﬁlms growing in random orientation. Another key observation is that SMCs’ contractile phenotype and ECM production might also be altered depending on synergistic eﬀect of surface wettability, surface chemistry, and substrate stiﬀness, as observed in case of the BMF group.
5. CONCLUSIONS Vascular pathologies are majorly associated with malfunction of vascular cells under the inﬂuence of dynamic microenvironment. Understanding the functional aspect of these cells under in vitro conditions demands the recapitulation of native-like environment involving multiple physicochemical factors. In this work, we evaluated the functionality of vascular cells (SMCs and ECs) cultured on engineered silk ﬁlm surfaces having diﬀerent wettability, roughness, chemistry and mechanical stiﬀness owing to variable inherent characteristics of BM and AA silk. Our ﬁndings suggest that surface pattern induced alignment solely is not adequate for maintaining ECs’ functionality; however other surface properties play a crucial role. For instance, ECs’ showed superior proliferation on AA ﬁlms irrespective of their surface patterning. On the other hand, gene expression proﬁle and NO quantiﬁcation data evidenced the negative impact of surface pattern induced cellular alignment. In contrast, SMCs were more responsive when cultured on patterned surfaces in terms of proliferation, expression of contractile genes, remodeling capability and physical contraction. Surface patterning favorably induced the unidirectional cell alignment and modulated their function. Together with surface patterning, other surface properties of ﬂat silk ﬁlms (BMF) also inﬂuenced the contractile gene expression and ECM production favorably. Altogether, this study demonstrates that surface physicochemical properties of silk ﬁlms synergistically determine the functional behavior of vascular cells.
S Supporting Information *
The Supporting Information is available free of charge on the ACS Publications website at DOI: 10.1021/acsbiomaterials.8b01194.
Schematic representation of direction of contact angle measurement for patterned silk ﬁlms, load−displacement curves of silk ﬁlms, marker expression by vascular cells, lower magniﬁcation images of vascular cells cultured on silk ﬁlms (PDF)
activations by prostacyclin released by sheared endothelial cells. Circ. Res. 2009, 105 (5), 471−480. (15) Cao, Y.; Poon, Y. F.; Feng, J.; Rayatpisheh, S.; Chan, V.; ChanPark, M. B. Regulating orientation and phenotype of primary vascular smooth muscle cells by biodegradable films patterned with arrays of microchannels and discontinuous microwalls. Biomaterials 2010, 31 (24), 6228−6238. (16) Webb, K.; Hlady, V.; Tresco, P. A. Relationships among cell attachment, spreading, cytoskeletal organization, and migration rate for anchorage-dependent cells on model surfaces. J. Biomed. Mater. Res. 2000, 49 (3), 362. (17) Kessler, F.; Steffens, D.; Lando, G. A.; Pranke, P.; Weibel, D. E. Wettability and cell spreading enhancement in poly (sulfone) and polyurethane surfaces by UV-assisted treatment for tissue engineering purposes. Tissue Eng. Regener. Med. 2014, 11 (1), 23−31. (18) Bacakova, L.; Filova, E.; Parizek, M.; Ruml, T.; Svorcik, V. Modulation of cell adhesion, proliferation and differentiation on materials designed for body implants. Biotechnol. Adv. 2011, 29 (6), 739−767. (19) Shen, Y.; Gao, M.; Ma, Y.; Yu, H.; Cui, F.z.; Gregersen, H.; Yu, Q.; Wang, G.; Liu, X. Effect of surface chemistry on the integrin induced pathway in regulating vascular endothelial cells migration. Colloids Surf., B 2015, 126, 188−197. (20) Brown, X. Q.; Ookawa, K.; Wong, J. Y. Evaluation of polydimethylsiloxane scaffolds with physiologically-relevant elastic moduli: interplay of substrate mechanics and surface chemistry effects on vascular smooth muscle cell response. Biomaterials 2005, 26 (16), 3123−3129. (21) Ren, X.; Feng, Y.; Guo, J.; Wang, H.; Li, Q.; Yang, J.; Hao, X.; Lv, J.; Ma, N.; Li, W. Surface modification and endothelialization of biomaterials as potential scaffolds for vascular tissue engineering applications. Chem. Soc. Rev. 2015, 44 (15), 5680−5742. (22) Chung, T. W.; Liu, D. Z.; Wang, S. Y.; Wang, S. S. Enhancement of the growth of human endothelial cells by surface roughness at nanometer scale. Biomaterials 2003, 24 (25), 4655− 4661. (23) Xu, C.; Yang, F.; Wang, S.; Ramakrishna, S. In vitro study of human vascular endothelial cell function on materials with various surface roughness. J. Biomed. Mater. Res. 2004, 71 (1), 154−161. (24) Choudhary, S.; Berhe, M.; Haberstroh, K. M.; Webster, T. J. Increased endothelial and vascular smooth muscle cell adhesion on nanostructured titanium and CoCrMo. International journal of nanomedicine 2006, 1 (1), 41. (25) Trappmann, B.; Gautrot, J. E.; Connelly, J. T.; Strange, D. G.; Li, Y.; Oyen, M. L.; Stuart, M. A. C.; Boehm, H.; Li, B.; Vogel, V.; et al. Extracellular-matrix tethering regulates stem-cell fate. Nat. Mater. 2012, 11 (7), 642. (26) Gupta, P.; Hari Narayana S. N., G.; Kasiviswanathan, U.; Agarwal, T.; Senthilguru, K.; Mukhopadhyay, D.; Pal, K.; Giri, S.; Maiti, T. K.; Banerjee, I. Substrate stiffness does affect the fate of human keratinocytes. RSC Adv. 2016, 6 (5), 3539−3551. (27) Gupta, P.; Kumar, M.; Bhardwaj, N.; Kumar, J. P.; Krishnamurthy, C.; Nandi, S. K.; Mandal, B. B. Mimicking form and function of native small diameter vascular conduits using mulberry and non-mulberry patterned silk films. ACS Appl. Mater. Interfaces 2016, 8 (25), 15874−15888. (28) Bhunia, B. K.; Kaplan, D. L.; Mandal, B. B. Silk-based multilayered angle-ply annulus fibrosus construct to recapitulate form and function of the intervertebral disc. Proc. Natl. Acad. Sci. U. S. A. 2018, 115 (3), 477−482. (29) Moses, J. C.; Nandi, S. K.; Mandal, B. B. Multifunctional Cell Instructive Silk-Bioactive Glass Composite Reinforced Scaffolds Toward Osteoinductive, Proangiogenic, and Resorbable Bone Grafts. Adv. Healthcare Mater. 2018, 7, 1701418. (30) Janani, G.; Nandi, S. K.; Mandal, B. B. Functional hepatocyte clusters on bioactive blend silk matrices towards generating bioartificial liver constructs. Acta Biomater. 2018, 67, 167.
The authors declare no competing ﬁnancial interest.
ACKNOWLEDGMENTS B.B.M. thankfully acknowledges the generous funding provided by Department of Biotechnology (DBT - BT/PR16605/NER/ 95/220/2015; BT/548/NE/U-Excel/2014; BT/PR22093/ NNT/28/1226/2017) and Department of Science and Technology (DST), Government of India. P.G. and J.C.M. acknowledge Ministry of Human Resource Development (MHRD) for fellowship. The contribution of Mr. Bibhas Kumar Bhunia for help with FESEM imaging is appreciated. The Central Instruments Facility (CIF) and Department of Biosciences and Bioengineering, IIT Guwahati are also acknowledged for providing high-end instruments.
(1) Barthes, J.; Ö zçelik, H.; Hindié, M.; Ndreu-Halili, A.; Hasan, A.; Vrana, N. E. Cell Microenvironment Engineering and Monitoring for Tissue Engineering and Regenerative Medicine: The Recent Advances. BioMed Res. Int. 2014, 2014, 921905. (2) Kim, D. H.; Provenzano, P. P.; Smith, C. L.; Levchenko, A. Matrix nanotopography as a regulator of cell function. J. Cell Biol. 2012, 197 (3), 351−360. (3) Bhadriraju, K.; Chen, C. S. Engineering cellular microenvironments to improve cell-based drug testing. Drug Discovery Today 2002, 7 (11), 612−620. (4) Warren, K. M.; Islam, M. M.; LeDuc, P. R.; Steward, R., Jr 2D and 3D mechanobiology in human and nonhuman systems. ACS Appl. Mater. Interfaces 2016, 8 (34), 21869−21882. (5) Bettinger, C. J.; Langer, R.; Borenstein, J. T. Engineering substrate topography at the micro-and nanoscale to control cell function. Angew. Chem. Int. Ed. 2009, 48 (30), 5406−5415, DOI: 10.1002/anie.200805179. (6) Alford, P. W.; Nesmith, A. P.; Seywerd, J. N.; Grosberg, A.; Parker, K. K. Vascular smooth muscle contractility depends on cell shape. Integrative Biology 2011, 3 (11), 1063−1070. (7) Sinha, R.; Le Gac, S.; Verdonschot, N.; Van Den Berg, A.; Koopman, B.; Rouwkema, J. Endothelial cell alignment as a result of anisotropic strain and flow induced shear stress combinations. Sci. Rep. 2016, 6, 29510. (8) Choi, J. S.; Piao, Y.; Seo, T. S. Circumferential alignment of vascular smooth muscle cells in a circular microfluidic channel. Biomaterials 2014, 35 (1), 63−70. (9) Thakar, R. G.; Ho, F.; Huang, N. F.; Liepmann, D.; Li, S. Regulation of vascular smooth muscle cells by micropatterning. Biochem. Biophys. Res. Commun. 2003, 307 (4), 883−890. (10) Li, W.; Chen, J.; Xu, P.; Zhu, M.; Wu, Y.; Wang, Z.; Zhao, T.; Cheng, Q.; Wang, K.; Fan, G.; et al. Long-term evaluation of vascular grafts with circumferentially aligned microfibers in a rat abdominal aorta replacement model. J. Biomed. Mater. Res., Part B 2018, 106, 2596. (11) Zhu, M.; Wang, Z.; Zhang, J.; Wang, L.; Yang, X.; Chen, J.; Fan, G.; Ji, S.; Xing, C.; Wang, K.; et al. Circumferentially aligned fibers guided functional neoartery regeneration in vivo. Biomaterials 2015, 61, 85−94. (12) Rajendran, P.; Rengarajan, T.; Thangavel, J.; Nishigaki, Y.; Sakthisekaran, D.; Sethi, G.; Nishigaki, I. The vascular endothelium and human diseases. Int. J. Biol. Sci. 2013, 9 (10), 1057. (13) Wang, Z.; Teoh, S. H.; Hong, M.; Luo, F.; Teo, E. Y.; Chan, J. K. Y.; Thian, E. S. Dual-microstructured porous, anisotropic film for biomimicking of endothelial basement membrane. ACS Appl. Mater. Interfaces 2015, 7 (24), 13445−13456. (14) Tsai, M. C.; Chen, L.; Zhou, J.; Tang, Z.; Hsu, T. F.; Wang, Y.; Shih, Y. T.; Peng, H. H.; Wang, N.; Guan, Y.; et al. Shear stress induces synthetic-to-contractile phenotypic modulation in smooth muscle cells via peroxisome proliferator-activated receptor α/δ O
ACS Biomaterials Science & Engineering (31) Konwarh, R.; Bhunia, B. K.; Mandal, B. B. Opportunities and Challenges in Exploring Indian Non-mulberry Silk for Biomedical Applications. Proc. Indian Natn Sci. Acad. 2017, 83, 85−101. (32) Gupta, A.; Mita, K.; Arunkumar, K. P.; Nagaraju, J. Molecular architecture of silk fibroin of Indian golden silkmoth, Antheraea assama. Sci. Rep. 2015, 5, 12706. (33) Asakura, T.; Yao, J.; Yamane, T.; Umemura, K.; Ulrich, A. S. Heterogeneous Structure of Silk Fibers from Bombyx M Ori Resolved by 13C Solid-State NMR Spectroscopy. J. Am. Chem. Soc. 2002, 124 (30), 8794−8795. (34) Zhou, C. Z.; Confalonieri, F.; Medina, N.; Zivanovic, Y.; Esnault, C.; Yang, T.; Jacquet, M.; Janin, J.; Duguet, M.; Perasso, R. Fine organization of Bombyx mori fibroin heavy chain gene. Nucleic acids research 2000, 28 (12), 2413−2419. (35) Lefèvre, T.; Rousseau, M.-E.; Pézolet, M. Protein secondary structure and orientation in silk as revealed by Raman spectromicroscopy. Biophys. J. 2007, 92 (8), 2885−2895. (36) Bratzel, G.; Buehler, M. J. Sequence-structure correlations in silk: Poly-Ala repeat of N. clavipes MaSp1 is naturally optimized at a critical length scale. Journal of the mechanical behavior of biomedical materials 2012, 7, 30−40. (37) Gil, E. S.; Mandal, B. B.; Park, S.-H.; Marchant, J. K.; Omenetto, F. G.; Kaplan, D. L. Helicoidal multi-lamellar features of RGD-functionalized silk biomaterials for corneal tissue engineering. Biomaterials 2010, 31 (34), 8953−8963. (38) Lammel, A. S.; Hu, X.; Park, S.-H.; Kaplan, D. L.; Scheibel, T. R. Controlling silk fibroin particle features for drug delivery. Biomaterials 2010, 31 (16), 4583−4591. (39) Garidel, P.; Schott, H. Fourier-transform midinfrared spectroscopy for analysis and screening of liquid protein formulations. Bioprocess Int. 2006, 4 (6), 48−55. (40) Yang, Z.; Tu, Q.; Maitz, M. F.; Zhou, S.; Wang, J.; Huang, N. Direct thrombin inhibitor-bivalirudin functionalized plasma polymerized allylamine coating for improved biocompatibility of vascular devices. Biomaterials 2012, 33 (32), 7959−7971. (41) Xu, J. G.; Zhu, S. Y.; Heng, B. C.; Dissanayaka, W. L.; Zhang, C. F. TGF-β1-induced differentiation of SHED into functional smooth muscle cells. Stem Cell Res. Ther. 2017, 8 (1), 10. (42) Lu, Q.; Hu, X.; Wang, X.; Kluge, J. A.; Lu, S.; Cebe, P.; Kaplan, D. L. Water-insoluble silk films with silk I structure. Acta Biomater. 2010, 6 (4), 1380−1387. (43) Braun-Dullaeus, R. C.; Mann, M. J.; Sedding, D. G.; Sherwood, S. W.; von der Leyen, H. E.; Dzau, V. J. Cell Cycle−Dependent Regulation of Smooth Muscle Cell Activation. Arterioscler., Thromb., Vasc. Biol. 2004, 24 (5), 845−850. (44) Tousoulis, D.; Kampoli, A.-M.; Papageorgiou, T. N. P.; Stefanadis, C. The Role of Nitric Oxide on Endothelial Function. Curr. Vasc. Pharmacol. 2012, 10 (1), 4−18. (45) Xu, J.; Shi, G. P. Vascular wall extracellular matrix proteins and vascular diseases. Biochim. Biophys. Acta, Mol. Basis Dis. 2014, 1842 (11), 2106−2119. (46) Chang, S.; Song, S.; Lee, J.; Yoon, J.; Park, J.; Choi, S.; Park, J. K.; Choi, K.; Choi, C. Phenotypic modulation of primary vascular smooth muscle cells by short-term culture on micropatterned substrate. PLoS One 2014, 9 (2), e88089. (47) Vatankhah, E.; Prabhakaran, M. P.; Semnani, D.; Razavi, S.; Zamani, M.; Ramakrishna, S. Phenotypic modulation of smooth muscle cells by chemical and mechanical cues of electrospun tecophilic/gelatin nanofibers. ACS Appl. Mater. Interfaces 2014, 6 (6), 4089−4101. (48) Feng, J.; Chan-Park, M. B.; Shen, J.; Chan, V. Quick layer-bylayer assembly of aligned multilayers of vascular smooth muscle cells in deep microchannels. Tissue Eng. 2007, 13 (5), 1003−1012. (49) Jeon, H.; Tsui, J. H.; Jang, S. I.; Lee, J. H.; Park, S.; Mun, K.; Boo, Y. C.; Kim, D. H. Combined effects of substrate topography and stiffness on endothelial cytokine and chemokine secretion. ACS Appl. Mater. Interfaces 2015, 7 (8), 4525−4532. (50) Ding, Y.; Yang, Z.; Bi, C. W.; Yang, M.; Xu, S. L.; Lu, X.; Huang, N.; Huang, P.; Leng, Y. Directing vascular cell selectivity and
hemocompatibility on patterned platforms featuring variable topographic geometry and size. ACS Appl. Mater. Interfaces 2014, 6 (15), 12062−12070. (51) Zorlutuna, P.; Rong, Z.; Vadgama, P.; Hasirci, V. Influence of nanopatterns on endothelial cell adhesion: Enhanced cell retention under shear stress. Acta Biomater. 2009, 5 (7), 2451−2459. (52) Gasiorowski, J. Z.; Liliensiek, S. J.; Russell, P.; Stephan, D. A.; Nealey, P. F.; Murphy, C. J. Alterations in gene expression of human vascular endothelial cells associated with nanotopographic cues. Biomaterials 2010, 31 (34), 8882−8888. (53) Beamish, J. A.; He, P.; Kottke-Marchant, K.; Marchant, R. E. Molecular regulation of contractile smooth muscle cell phenotype: implications for vascular tissue engineering. Tissue Eng., Part B 2010, 16 (5), 467−491. (54) Van Wachem, P.; Hogt, A.; Beugeling, T.; Feijen, J.; Bantjes, A.; Detmers, J.; Van Aken, W. Adhesion of cultured human endothelial cells onto methacrylate polymers with varying surface wettability and charge. Biomaterials 1987, 8 (5), 323−328. (55) Van Wachem, P.; Beugeling, T.; Feijen, J.; Bantjes, A.; Detmers, J.; Van Aken, W. Interaction of cultured human endothelial cells with polymeric surfaces of different wettabilities. Biomaterials 1985, 6 (6), 403−408. (56) Lu, J.; Rao, M. P.; MacDonald, N. C.; Khang, D.; Webster, T. J. Improved endothelial cell adhesion and proliferation on patterned titanium surfaces with rationally designed, micrometer to nanometer features. Acta Biomater. 2008, 4 (1), 192−201. (57) Moffa, M.; Sciancalepore, A. G.; Passione, L. G.; Pisignano, D. Combined Nano-and Micro-Scale Topographic Cues for Engineered Vascular Constructs by Electrospinning and Imprinted MicroPatterns. Small 2014, 10 (12), 2439−2450. (58) Kämmerer, P.; Heller, M.; Brieger, J.; Klein, M.; Al-Nawas, B.; Gabriel, M. Immobilisation of linear and cyclic RGD-peptides on titanium surfaces and their impact on endothelial cell adhesion and proliferation. Eur. Cell Mater. 2011, 21, 364−372. (59) Yeh, Y. T.; Hur, S. S.; Chang, J.; Wang, K. C.; Chiu, J. J.; Li, Y. S.; Chien, S. Matrix stiffness regulates endothelial cell proliferation through septin 9. PLoS One 2012, 7 (10), e46889. (60) Golias, C.; Charalabopoulos, A.; Charalabopoulos, K. Cell proliferation and cell cycle control: a mini review. International journal of clinical practice 2004, 58 (12), 1134−1141. (61) Marx, S. O.; Totary-Jain, H.; Marks, A. R. Vascular smooth muscle cell proliferation in restenosis. Circ.: Cardiovasc. Interventions 2011, 4 (1), 104−111. (62) Gong, X.; Yao, J.; He, H.; Zhao, X.; Liu, X.; Zhao, F.; Sun, Y.; Fan, Y. Combination of flow and micropattern alignment affecting flow-resistant endothelial cell adhesion. Journal of the mechanical behavior of biomedical materials 2017, 74, 11−20. (63) Nakayama, K. H.; Surya, V. N.; Gole, M.; Walker, T. W.; Yang, W.; Lai, E. S.; Ostrowski, M. A.; Fuller, G. G.; Dunn, A. R.; Huang, N. F. Nanoscale patterning of extracellular matrix alters endothelial function under shear stress. Nano Lett. 2016, 16 (1), 410−419. (64) Sneddon, J. M.; Vane, J. R. Endothelium-derived relaxing factor reduces platelet adhesion to bovine endothelial cells. Proc. Natl. Acad. Sci. U. S. A. 1988, 85 (8), 2800−2804. (65) Kohn, J. C.; Zhou, D. W.; Bordeleau, F.; Zhou, A. L.; Mason, B. N.; Mitchell, M. J.; King, M. R.; Reinhart-King, C. A. Cooperative effects of matrix stiffness and fluid shear stress on endothelial cell behavior. Biophys. J. 2015, 108 (3), 471−478. (66) Chen, J.y.; Hu, M.; Zhang, H.; Li, B.c.; Chang, H.; Ren, K.f.; Wang, Y.b.; Ji, J. Improved Antithrombotic Function of Oriented Endothelial Cell Monolayer on Microgrooves. ACS Biomater. Sci. Eng. 2018, 4 (6), 1976−1985. (67) Shin, Y. M.; Shin, H. J.; Heo, Y.; Jun, I.; Chung, Y.-W.; Kim, K.; Lim, Y. M.; Jeon, H.; Shin, H. Engineering an aligned endothelial monolayer on a topologically modified nanofibrous platform with a micropatterned structure produced by femtosecond laser ablation. J. Mater. Chem. B 2017, 5 (2), 318−328. (68) Hakanpaa, L.; Sipila, T.; Leppanen, V. M.; Gautam, P.; Nurmi, H.; Jacquemet, G.; Eklund, L.; Ivaska, J.; Alitalo, K.; Saharinen, P. P
ACS Biomaterials Science & Engineering Endothelial destabilization by angiopoietin-2 via integrin β1 activation. Nat. Commun. 2015, 6, 5962. (69) Strobel, H. A.; Dikina, A. D.; Levi, K.; Solorio, L. D.; Alsberg, E.; Rolle, M. W. Cellular self-assembly with microsphere incorporation for growth factor delivery within engineered vascular tissue rings. Tissue Eng., Part A 2017, 23 (3−4), 143−155. (70) Bhattacharyya, A.; Lin, S.; Sandig, M.; Mequanint, K. Regulation of vascular smooth muscle cell phenotype in threedimensional coculture system by Jagged1-selective Notch3 signaling. Tissue Eng., Part A 2014, 20 (7−8), 1175−1187. (71) Yipeng, J.; Yongde, X.; Yuanyi, W.; Jilei, S.; Jiaxiang, G.; Jiangping, G.; Yong, Y. Microtissues Enhance Smooth Muscle Differentiation and Cell Viability of hADSCs for Three Dimensional Bioprinting. Front. Physiol. 2017, 8, 534. (72) Carthy, J. M.; Luo, Z.; McManus, B. M. WNT3A induces a contractile and secretory phenotype in cultured vascular smooth muscle cells that is associated with increased gap junction communication. Lab. Invest. 2012, 92 (2), 246. (73) Zempo, N.; Kenagy, R. D.; Au, Y. T.; Bendeck, M.; Clowes, M. M.; Reidy, M. A.; Clowes, A. W. Matrix metalloproteinases of vascular wall cells are increased in balloon-injured rat carotid artery. Journal of vascular surgery 1994, 20 (2), 209−217.